212 Ultra Clean Processing of Semiconductor Surfaces IX
chamber wall. A higher chemical reaction temperature of SPM can be explored through various
chemical ratios in POU mixing.
Figure 1 shows the highest (T2) reaction temperature can be found at an optimized mixing ratio of
sulfuric acid and hydrogen peroxide with fixed pre-mixing sulfuric acid temperature. On the other
hand, a higher than T2 chemical reaction temperature of SPM (T3) can be further reached by
increasing the pre-mixing sulfuric acid temperature. Table I indicates three different chemical
reaction temperatures of fresh-dispense SPM, T3>T2>T1, which were prepared to check wet clean
efficiency with different reaction time. A current HCl-based selective etching baseline is also
included to make a physical and electrical performance comparison with HCl-free SPM-only
Results and Discussion
Figure 2a shows a traditional HCl-based selective etching process with a narrow process window
inducing silicide damage. Using a 25-minute SPM-only etching process at temperature T1 prevents
silicide damage, but Pt residue can be found at specific areas, as shown in Figure 2b. However, by
using the SPM-only etching process at the higher T2 process condition, silicide damage is prevented
and the unreacted NiPt layer can be fully removed, as indicated in Figure 2c. These results
demonstrate a critical chemical reaction temperature of SPM needs to be reached to effectively
remove residual Pt. The sheet resistance comparison of the NiPt salicide between HCl-based and
SPM-only T2 selective etching condition (two wafers for each condition) is shown in Figure 3. The
SPM-only T2 selective metal etching process indicates lower and tighter sheet resistance distributions
at N+/P+ AA and poly areas in comparison to HCl-based etching.
Table II indicates increasing SPM chemical reaction temperature can effectively reduce selective etch
process time without leaving Pt residue. As compared with the traditional HCl-based process time (30
min.), the SPM-only T2 condition can reduce the process time by 33% (20 min.) while SPM-only at
the higher T3 temperature condition can reduce the process time by 66% (10 min.). The sheet
resistance comparison of the NiPt salicide between the SPM-only T2 and SPM-onlyT3 processes are
shown in Figure 4. These sheet resistance measurement data indicate a higher SPM chemical reaction
temperature is not only helpful to improve process throughput but also provides better uniformity and
tighter sheet resistance distribution.
The high temperature SPM-only T2 process was used to verify the selective metal etching process
performance on SiGe-strained PMOS transistors, as shown in Figure 5a. The preliminary results
indicate no damage found on SiGe-embedded polysilicon gate area, as indicated in Figure 5b. Figure
6 demonstrates comparable or better sheet resistance and uniformity performance on P+ poly and AA
between the HCl-based baseline and the SPM-only T2 process condition.
A high-temperature, fresh-dispense SPM-only process is reported and evaluated for the 45nm CMOS
NiPt salicide process with SiGe structures. The SPM-only processes with higher chemical reaction
temperature yield lower and tighter sheet resistance distributions and up to 66% process time
reduction. This SPM-only selective metal etching process is also proven to be compatible with PMOS
strained SiGe structures. The next step is to evaluate the process extendibility of the fresh-dispense
SPM-only process for the 32nm technology node.
The author would like to thank Steven Wang, Luke Chang, and Jeffery Butterbaugh at FSI
International for their facilitation of high temperature SPM experiments.
Solid State Phenomena Vols. 145-146 213
 P. S. Lee, K. L. Pey, D. Mangelinck, J. Ding, D. Z. Chi and L. Chan, IEEE Electron Device Letters 22(2001), p.561.
 A. Lauwers, J. Kittl, M. Van Dal et al, Materials Science and Engineering B, Vol 114-115(2004), p.29-41.
 K.M Tan, T.Y Liow, Lee RTP et al, Electron Device Letters, IEEE, Vol 28, Issue 10(2007), p905-908.
 F.K LeGoues, R. Rosenberg and B.S Meyerson, Appl. Phys. Lett, Vol 54, Issue 7(1989), p.644-646.
 C. Demeurisse, P. Verheyen, K. Opsomer, et al., Microelectronic Engineering, Vol 84, Issue 11(2007), p.2547-2551.
 T.J. Armar, J.Appl. Phys, Vol 92, Issue 12(2002), p.7193-7199.
 Cotton, Simon A., Chemistry of Precious Metals, Springer-Verlag, 1997.
 M. Pourbaix, Altas of Electrochemical Equilibrium in Aqueous Solutions, National Association of Corrosion Science,
Houston, TX (1974).
 K K. Christenson, E. Olson, N.P. Lee et al, Symposium on Ultra Clean Processing of Semiconductor Surfaces (UCPSS),
Figure 1: SPM chemical reaction temperature as a function of the mixing ratio of sulfuric acid and hydrogen peroxide.
Table I: Selective etch process test conditions.
Process Time 10 min. 20 min. 25min. 30min. 40min.
Baseline (HCl based) V V
SPM only - T1 V
SPM only - T2 V V
SPM only - T3 V V
a b c
Figure 2: a) NiPt salicide damage by HCl-based 40min process time; b) Pt residue found at specific area for SPM-only T1
process; c) No salicide attack and Pt residue found for SPM-only T2.
214 Ultra Clean Processing of Semiconductor Surfaces IX
N+ Poly P+ Poly
N+ AA P+ AA
Figure 3: Sheet resistance comparison between HCl-based baseline and SPM-only T2 at N+/P+ AA and Poly areas.
Table II. Pt residue window as a function of etching process time
Process Time 5 min. 10 min. 15min. 20min. 25min. 30min. 40min.
Baseline(HCl based) - - - - - OK NG
SPM only - T2 - - NG OK OK - -
SPM only - T3 NG OK OK OK - - -
NG: Pt residue or salicide damage; OK: No Pt residue and damage free
N+ Poly P+ Poly
N+ AA P+ AA
Figure 4: Sheet resistance comparison between SPM-only T2 and SPM-only T3 at N+/P+ AA and Poly areas
Figure 5: a) PMOS with SiGe structure; b) No salicide attack and Pt residue found for SPM-only T2 at SiGe areas.
Figure 6: Sheet resistance comparison between HCl-based baseline and SPM-only T2 at N+/P+ AA and Poly areas.
Solid State Phenomena Vols. 145-146 215
Ultra Clean Processing of Semiconductor Surfaces IX
Advances on 45nm SiGe-Compatible NiPt Salicide Process